Home > Documents > MATHEMATICAL MODELING OF SOLIDIFICATION PHENOMENA …

MATHEMATICAL MODELING OF SOLIDIFICATION PHENOMENA …

Date post: 28-Mar-2022
Category:
Author: others
View: 0 times
Embed Size (px)
of 119 /119
MATHEMATICAL MODELING OF SOLIDIFICATION PHENOMENA IN ELECTROMAGNETICALLY STIRRED MELTS by GREGORY MICHAEL POOLE LAURENTIU NASTAC, COMMITTEE CHAIR MARK L. WEAVER HEATH TURNER AMBER GENAU CHARLES A. MONROE A DISSERTATION Submitted in partial fulfillment of the requirements for the degree of Doctor of Philosophy in the Department of Metallurgical and Materials Engineering in the Graduate School of The University of Alabama TUSCALOOSA, ALABAMA 2014
Transcript
ELECTROMAGNETICALLY STIRRED MELTS
for the degree of Doctor of Philosophy in the
Department of Metallurgical and Materials Engineering
in the Graduate School of
The University of Alabama
ii
ABSTRACT
A methodology is presented to simulate the electromagnetic, heat transfer, and fluid flow
phenomena for two dimensional electromagnetic solidification processes. For computation of the
electromagnetic field, the model utilizes the mutual inductance technique to limit the solution
domain to the molten metal and magnetic shields, commonly present in solidification systems.
The temperature and velocity fields were solved using the control volume method in the metal
domain. The developed model employs a two domain formulation for the mushy zone.
Mathematical formulations are presented for turbulent flow in the bulk liquid and the suspended
particle region, along with rheological behavior. An expression has been developed—for the first
time—to describe damping of the flow in the suspended particle region as a result of the
interactions between the particles and the turbulent eddies. The flow in the fixed particle region
is described using Darcy’s law. Calculations were carried out for globular and dendritic
solidification morphologies of an electromagnetically-stirred melt in a bottom-chill mold. The
coherency solid fraction for the globular solidification morphology was taken to be 0.5, while the
coherency for dendritic morphology was 0.25. The results showed the flow intensity in the
suspended particle region was reduced by an order of magnitude. The effect of the heat
extraction rate on solidification time was investigated using three different heat transfer
coefficients. The results showed that the decrease in solidification time is nonlinear with respect
to increasing heat transfer coefficient. The influence of the final grain size on the damping of the
iii
flow in the suspended particle region was examined, and it was found that larger grain sizes
reduce the extent of flow damping.
iv
A Magnetic vector potential
B Magnetic flux density
Dm Molecular mass diffusivity
d Instantaneous grain size
dl Differential line element
vi
L Latent heat of fusion
Mij Mutual inductance
RT Turbulent Reynolds number
∇ Del operator
µm Molecular viscosity
µl Laminar viscosity
τt Turbulent (Reynolds) Stress
ψ Magnetic scalar potential
ω Angular frequency
ix
ACKNOWLEDGEMENTS
When I began composing this dissertation, I would have never imagined that I would
complete my studies without a man who, in the end, not only guided me in my acquisition of
knowledge, but also became a dear friend. Professor Nagy El-Kaddah was a the best person I
could have ever asked for in a research advisor. He and I would not only discuss the fundamental
phenomena that governs the world in which we live, but would also delve into the very heart of
issues of philosophy and the human condition. I cannot imagine where I would be today had he
not mentored me in both my undergraduate years as a student and later as his pupil, and I only
hope to be half of the mentor he was to me to others. Unfortunately, his time was cut short, and
his no longer being among us is a tragedy of the greatest kind. Both the University of Alabama
and I will greatly miss him.
I would first like to express my gratitude to my other advisor, Dr. Laurentiu Nastac, who
took the reins amidst a difficult situation and guided me to further my career goals. I would also
like to thank the National Science Foundation for affording the great privilege to complete this
work under grant number CMMI-0856320. I would also like thank the members of my defense
committee, Drs. Mark L. Weaver, Heath Turner, Amber Genau and Charles A. Monroe for
taking the time to offer their insights and suggestions on this project.
In addition to those who have been instrumental in directly offering their guidance in this
work, prudence dictates that gratitude be expressed for those who have made indelible
impressions on my career. Professor David Nikles has been my greatest supporter at the
University of Alabama, beginning with my interning in his research lab within the Center for
Materials for Information Technology developing magnetic data storage materials—an
x
internship that led me to devote my learning and explaining the world around us to others. I
would also like to thank my high school mathematics teachers, Ms. Vanetta Clark, Mrs. Betty
Trayvick, Mrs. Susan Copen, and Mrs. Elaine Noland, whose instruction inspired me to gain and
apply my mathematical knowledge to the benefit of others. Most importantly, I thank my father,
Michael, and my mother, Susan, for supporting my endless quest for knowledge, and for their
constant consolation and encouragement along the way.
Finally, I must acknowledge the pillar and foundation of truth, whose truth I am merely
rediscovering—Veritas Christo et Ecclesiae.
xi
CONTENTS
ACKNOWLEDGEMENTS ....................................................................... ix
2.2.1 Isothermal Solidification ...................................................................12
2.3.1 Single-zone Models ..........................................................................17
2.3.2 Dual-zone Models .............................................................................19
2.4 Modeling of Solute Segregation during Solidification ........................21
Chapter 3. An Improved Model for the Flow in an Electromagnetically
Stirred Melt during Solidification ..............................................................24
3.6 Conclusions ..........................................................................................43
3.7 Acknowledgements ..............................................................................45
3.8 References ............................................................................................45
Appendix 3A: The Damping Force in the Suspended Particle Region .....48
Chapter 4. The Effect of Coil Design on the Temperature and Velocity
Fields during Solidification in Electromagnetic Stirring Processes ..........49
4.1 Abstract ................................................................................................49
4.2 Introduction ..........................................................................................50
4.3.2 Formulation of the Heat Transfer Problem .......................................53
4.3.3 Formulation of the Fluid Flow Problem ...........................................54
4.3.4 Turbulent Damping Model ...............................................................55
Solidifying in the Presence of Electromagnetic Stirring............................68
5.1 Abstract ................................................................................................68
5.2 Introduction ..........................................................................................68
5.5 Conclusions ..........................................................................................86
5.6 References ............................................................................................87
6.1 Concluding Remarks ............................................................................91
References ..................................................................................................92
xiv
5.1 Thermophysical properties used in the present study ..........................74
xv
3.2 Flow domains for the dual-zone solidification model .........................28
3.3 Dimensions of the system used in this study .......................................32
3.4 Computed Lorentz (EM) force field in the metal and chill block........34
3.5 Computed vorticity of the EM force field in the metal ........................35
3.6 Initial characteristics of the flow: (a) velocity and (b) turbulent-to-
laminar viscosity ratio ................................................................................36
3.7 Computed velocity profiles in the metal at: (a) 30s, (b) 60s, (c) 120s,
(d) 240s. Contours correspond to values of solid fraction .........................37
3.8 Computed turbulent-to-laminar viscosity in the metal at: (a) 30s, (b)
60s, (c) 120s, (d) 240s ................................................................................39
3.9 Comparison between the velocity in the suspended particle region
with and without damping force ................................................................40
3.10 Comparison of turbulence in the suspended particle region with and
without damping force ...............................................................................41
3.11 Influence of final grain size, Dg, on damping of velocity in the
suspended particle region ...........................................................................41
3.12 Influence of final grain size, Dg, on damping of turbulence in the
suspended particle region ...........................................................................42
4.1 Sketch of unidirectional EM solidification system ..............................56
4.2 Initial flow patterns at different coil locations: (a) middle, (b) top,
and (c) bottom ............................................................................................58
4.3 Initial turbulent fields at different coil positions: (a) middle, (b) top,
and (c) bottom ............................................................................................59
4.4 Computed velocity and temperature fields in the suspended particle
region after 120s: (a) middle, (b) top, and (c) bottom coil positions .........61
4.5 A comparison of the radial temperature distributions for the top and
bottom coil positions after 120s (z=20 mm) ..............................................62
xvi
4.6 Decay of velocity in the suspended particle region for top and
bottom coil positions (r=20 mm, z=30 mm) ..............................................63
4.7 Decay of turbulent-to-laminar viscosity ratio in the suspended
particle region for top and bottom coil positions (r=20 mm, z=30 mm) ...64
5.1 Flow domains for the dual-zone solidification model .........................70
5.2 Dimensions of the system used in this study .......................................75
5.3 Initial computed velocity field .............................................................75
5.4 Initial turbulent field given in terms of turbulent-to-molecular
viscosity .....................................................................................................76
5.5 Damping of the velocity and turbulent fields. Data taken at the
centerline 20 mm from the chill .................................................................77
5.6 Computed velocity and liquid solute profile after 360s for
frequency of 4900 Hz.................................................................................78
5.7 Solute segregation profile after 550s. Note the change of scale in the
velocity .......................................................................................................79
5.8 Axial liquid concentration profiles, taken at the centerline for
different stages of solidification.................................................................80
5.9 Electron backscatter micrographs taken for EM stirred sample at
(a) 20 mm and (b) 60 mm from chill block. Images taken at ingot
centerline ....................................................................................................80
with experimental measurements ...............................................................81
5.11 Influence of assumed fs vs T profile on the final solute
composition at the centerline .....................................................................82
5.12 Influence of final grain size on the final centerline composition .......83
5.13 Effect of frequency on centerline segregation ...................................84
5.14 Velocity and liquid solute concentration field after 360 seconds for
frequency of 500 Hz...................................................................................84
In the past several decades, electromagnetic (EM) induction stirring technologies have
become an attractive means to achieve a fine-grained equiaxed structure in solidification
processes. In EM stirring, an alternating current is passed through a suitable induction coil; this,
in turn, generates eddy currents within the molten metal. These eddy currents then interact with
the time-varying magnetic field generated by the coil to generate stirring (Lorentz) forces, the
rotational component of which drives the flow. This ability to produce an “action at a distance”
by generating flows without any physical contact with the melt—often a cause of
contamination—makes EM stirring uniquely useful in a number of solidification processes. To
this end, examples of EM stirring being utilized during solidification include continuous casting
[1-3], direct chill (DC) casting [4, 5], suspension melting [6, 7], and semiconductor processing
using Bridgeman furnaces [8, 9].
In most cases, the flows generated by EM stirring are very intense and highly turbulent;
this causes the convective phenomena in the melt to exert a dominating influence on the micro-
and macrostructural evolution of the cast alloy, particularly in the early stages of solidification.
The influences of EM stirring flows on the solidification are well-documented in the
experimental literature and are manifold in scope. In the bulk liquid, the flow serves to promote
homogeneous solute and temperature fields in the melt [10-12]. Furthermore, the flow causes the
superheat in the melt to dissipate rapidly due to the increased Nusselt number near the chill
interface, facilitating a greater nuclei survival probability [13] and uniform growth kinetics [14,
15]. As solidification commences and a two-phase “mushy” region forms, the flow continues to
2
minimize the temperature gradient between the solid crystallites and the surrounding liquid [16],
promoting an earlier occurrence of the columnar-to-equiaxed transition in the cast alloy [17].
However, the greatest contribution of EM stirring to grain refinement comes via the dendrite
fragmentation mechanism, first proposed by Jackson and co-workers [18] and confirmed through
in situ experiments [19-21]. In dendrite fragmentation, flow between coalesced dendrites
transports, or “washes”, solute-enriched liquid from deep within the mushy region to the solid-
liquid interface. This causes the secondary dendrite arms at the interface to undergo remelting,
and the detached tips are then carried into the liquid, increasing the nucleation potential of the
melt and thus reducing the grain size.
In addition to micro- and macrostructural changes induced by EM stirring, the flow also
has a profound effect on the distribution of solute in the mushy region, commonly referred to as
“segregation”. Indeed, it has been repeatedly shown on the macroscale that, depending on the
type of field used, the solute profiles within the solidified cast alloy vary greatly depending on
the flow characteristics, which themselves depend on the type of magnetic field used, the most
common of which are stationary [3, 22], rotating [23], and traveling magnetic fields [24]. On the
microscale, the flow modifies the extent of solute rejection, represented by the partition
coefficient [25].
This creates an imperative to understand the flow characteristics in both the melt and
mushy regions in order to ensure adequate control of the solidification phenomena within the
cast alloy. To this end, the development and implementation of mathematical modeling tools
provides an attractive and economical alternative to incessant experimentation; however, these
developed tools, while useful, are only as reliable if the physical phenomena that the model
intends to reflect are well-defined. Therefore, it is vital that all aspects of electromagnetic, heat
3
transfer, fluid flow, and mass transfer phenomena in both the bulk liquid and mushy regions
must be accounted for if a rigorous solution is to be obtained for any EM stirred solidification
system.
Previous work, exemplified by those of Evans [26, 27], Szekely [21, 28], and El-Kaddah
[29, 30], have led to a good fundamental understanding of the phenomena involved in EM
stirring of bulk liquids. Their approach involves the solution of the Maxwell equations for the
electromagnetic field and the turbulent Navier-Stokes equations in the bulk liquid. However,
implementation of the methods described in the references above becomes more cumbersome
when considering two-phase flows.
There have been a number of approaches developed to describe the flow in the mushy
region. Initial efforts involved treating the mushy region as a porous medium governed by
Darcy’s law [31-34], along with supplementary relations for describing the flow permeability
[35, 36]. It is important to note that these models, which assume stationary crystallites, are only
suitable to either laminar buoyancy-driven or shrinkage-driven flows during; however, there
have been some efforts to incorporate turbulent flow behavior [37, 38]. Furthermore, such flows
are physically valid for columnar solidification only, as equiaxed grains travel with the flow at
low fraction solid [18-20].
To remedy this, a new model, introduced by Oldenburg and Spera [39], relaxes the
porous medium assumption at low fraction solid, replacing it with a homogeneous two-phase
flow formulation where the viscosity of the solid-liquid mixture is described by rheological
behavior. The Darcy flow assumption is maintained at higher fraction solid, with the two flow
domains being delineated by the coherency fraction solid, defined as when the growing
crystallites first begin to impinge on one another. Other variations of the dual-zone model have
4
been presented. Beckermann and coworkers [40] have presented a volume-averaged two-phase
flow model to determine the velocities of both the solid and liquid phases at low fraction solid,
and Nikrityuk et al [41] assumed rheological behavior over the entire mushy region. However,
each of these formulations assumed laminar flow in both the bulk liquid and mushy regions.
Recently, Pardeshi et al extended this the hybrid flow model to describe solidification in the
presence of turbulent flow [42]. In this model, the k-ε model to describe the turbulent
characteristics in the bulk liquid and at low fraction solid. However, the model does not account
for flow damping via the interaction of the turbulent eddies and the solid crystallites. This
interaction has been experimentally shown to have a key role in damping the flow intensity in the
liquid phase, and must be considered in the analysis to accurately predict the liquid velocity, and
due to the strong coupling between the flow and other transport variables, the extent of solute
segregation and the temperature gradient.
Previous work by the author [43] led to the development of a rudimentary formulation for
describing the flow damping by the turbulent crystallite interactions in the mushy region. In this
model, an equivalent damping point force was derived by assuming homogeneous turbulence,
with the force being described in terms of the turbulent kinetic energy, the fraction solid, and the
coherency fraction solid. Although the results were consistent with expectations, the model had
several pitfalls, particularly with respect to the direction in which the point force was applied,
which was assumed to be invariant.
The endeavor of this research will be on developing realistic modeling tools for
describing the electromagnetic, temperature, concentration, and velocity fields in EM stirred
processes during solidification. The goals may be succinctly stated as follows:
5
(1) To develop a methodology for describing the contribution of turbulence in damping
the flow in the mushy zone.
(2) To develop a methodology that solves the electromagnetic field and the conservation
equations for temperature, solute concentration, and fluid flow in solidification processes.
(3) To investigate the effect of solidification parameters, namely the crystallite size and
solidification morphology, on the flow behavior in the bulk and mushy zone during
solidification.
(4) To determine the model’s capability to accurately predict the solute segregation
patterns found by experiments.
(5) To determine the effect of the flow characteristics on the extent and pattern of
macrosegregation in the mushy region during solidification.
(6) To determine the effects of induction coil design, namely the coil position and
configuration, on the pattern and intensity of the flow in both the bulk liquid and the
mushy region.
This dissertation will proceed as follows:
Chapter two will provide a review of techniques used in literature for describing
the electromagnetic, heat transfer, fluid flow, and solute segregation phenomena
in EM stirred solidification systems.
Chapter three will present a manuscript published in Metallurgical and Materials
Transactions B [44] which describes the basic formulation used in this study
along with preliminary results.
6
Chapter four will present a manuscript published in ISIJ International [45] that
employs this model presented in Chapter 3 in discussing the influence of key coil
design parameters on the solidification behavior.
Chapter five will present a manuscript submitted to the International Journal of
Cast Metals Research that will expand the model presented in Chapter three to
determine the effects of the turbulent damping model to solute segregation and
compare the computed results with experimental measurements.
Chapter six will briefly review the principal findings of these research studies,
along with several suggestions for future research topics which may be further
explored at a later date.
7
Chapter 2
Literature Review
There has been significant progress made in simulation techniques for describing the
electromagnetic, fluid flow, heat transfer, and mass transfer phenomena in solidification
processes. This chapter will provide an overview of previously published literature on numerical
simulation of the electromagnetic, temperature, solute, and velocity fields in solidification
systems.
The electromagnetic field quantities are governed by the Maxwell equations. Namely,
these are the differential formulations of the integral Gauss laws for conservation of the electric
and magnetic fields, Ampere’s law for describing the relationship between the electric current
and the magnetic field, and Faraday’s law of induction. The flow characteristics in EM stirred
systems strongly depend on the type of field used. The most commonly used are stationary [3,
22], rotating [34, 41, 42], and traveling magnetic fields [22, 30].
Although the discussion of literature will be focused primarily on solving the
electromagnetic field numerically, it is necessary to note for the purposes of rigor that a majority
of models for EM solidification systems have employed approximate analytical solutions [38, 42,
46-48] for describing the resulting Lorentz force field in the melt. While such solutions are
simple to implement and saves computing time for solving the EM field in the molten metal,
they suffer from several drawbacks. First, these solutions may only be obtained for highly
simplified infinite or semi-infinite systems possessing a significant degree of symmetry, making
them untenable for more complex, finite geometries. This is especially made clear for rotary
8
stirring, where Davidson and Boysan [49] examined the flow in rotary stirring of round billet
castings. They found that the flow induced in the round is a superposition of the primary,
rotational flow resulting from the applied rotating field and a secondary, axial flow driven by the
gradient of the EM force near the top and bottom boundaries of the stirrer. This is made even
clearer by the work of Schwerdtfeger and colleagues [48] on modeling idealized continuous
casting systems. By simplifying the EM field problem to two dimensions, only the primary flow
field in the molten pool was resolved. The secondary flow field predicted by Davidson and
Boysan [49] was later confirmed by Meyer et al [3], who solved the EM field problem
numerically for finite sized continuous casting systems.
Secondly, the assumptions made for approximate analytical solutions made them ill-
suited to accommodate the presence of adjacent conducting materials, which act as magnetic
shields and distort the magnetic flux lines around the induction coil. This leads to variations of
the Lorentz force within the molten metal, changing the flow pattern. An example of this may be
found in the work of Vives and Ricou [50], who examined the effect of placing copper magnetic
shields on the flow structure in a coreless induction furnace.
This articulates the need for a numerical solution to the EM field problem. Most
computational techniques for numerically computing the EM field quantities are based on
solving the differential forms of the Maxwell equations based on potential formulations for the
electric field, E, and the magnetic field, B. Use of potentials allows for simplified handling of the
boundary conditions and discontinuities in the tangential component of the electric field and the
normal component of the magnetic field. Potentials may be generally classified into two types:
(i) scalar potentials and (ii) vector potentials. The most frequently used scalar potentials in
formulations alternating EM field problems are the electric scalar potential, V, and the reduced
9
magnetic scalar potential, ψ. Similarly, the most common vector potentials are the magnetic
vector potential, A, and the current vector potential, T. The differential equations using scalar
potentials are of Laplace-Poisson type, while the governing vector potential equations are
diffusion-type for eddy current problems.
Most formulations for eddy current problems have been primarily based on the magnetic
vector potential. Roger and Eastham [51] used the vector potential A for the field conductor,
along with scalar potentials, namely ψ for free space and for ferromagnetic materials, in the
non-conducting media. The Biot-Savart law was used to describe the source fields (i.e. from the
coil). While this does allow for a solution to be obtained, this method suffers from two principal
drawbacks. First, this method only works for singly-connected conducting domains, meaning
that it cannot accommodate the presence of magnetic shields. Furthermore, the method requires
that the domain have uniform electrical conductivity, which is not physically valid during
solidification.
The remedy to the latter problem was put forth by Pillsbury [52], who introduced the
A,V- formulation to allow for variable electrical conductivity. In that work, the magnetic and
electric fields by solving for A and V, respectively, with being used to determine the field in
free space. However, the use of the magnetic scalar potential in free space means that this
method still does not allow for magnetic shields. To remedy the magnetic shield drawback,
Roger et al [53] proposed a form of domain decomposition by using cuts in the conductor in the
direction of the current. However, implementation of this proposal requires special routines to
deal with discontinuities at the domain boundaries, increasing the computational complexity of
the problem. The multiply-connected domain problem was remedied by both Chari et al [54] and
Biddlecombe et al [55], who both introduced the A,V-A formulation. This allows for the
10
presence of multiple conductors in the overall solution domain without the need for stiff current
sources—the assumption that the induced currents do not influence the source current—at the
cost of increased degrees of freedom.
The use of the current vector potential appeared in the literature more recently, with
Carpenter et al [56-58] first suggesting such a formulation. Preston et al [59] was the first to use
the T-ψ,ψ formulation. Here the current vector potential was used to solve the eddy current
distribution within the conductor, and the magnetic field was represented by the reduced scalar
potential. To enforce continuity of the current vector potential at the boundaries, a gauge
condition was used, meaning that the formulation can be applied to problems involving multiply-
connected domains. The computational advantages associated with various magnetic and current
vector potential formulations were investigated by Reinhart [60] and Biro [61].
Solutions of the differential equations are generally carried out using the finite element
method, finite difference method, or the control volume techniques. For further details, the
reader may refer to References [62-64]. The principal drawback with these solution methods is
that eddy current problems are open bounded in nature, meaning that the solution domain must
not only include the conducting regions, but free space as well in order to properly define the
boundary conditions of the solution domain, causing significant computational inefficiency.
This drawback may be remedied through the use of hybrid techniques. These techniques
employ two different solution methods in such a way that the weakness of one solution method is
compensated by the strength of the counterpart method. In the hybrid boundary element/FEM
technique of Salon [65], the differential vector potential equation is solved using the finite
element method, while the boundary element method is used to resolve the boundary conditions.
El-Kaddah and coworkers [66] used the control volume/integral method. In this procedure, the
11
control volume technique is used to solve the magnetic diffusion equation for A within the
conductor, while the boundary conditions are resolved using the Biot-Savart law. An analogous
procedure was developed using the finite element method by El-Kaddah and Natarajan [67, 68].
These hybrid methods were later shown to be more computationally efficient than any of the
various standalone methods [69].
In two dimensional systems or three dimensional ones possessing a symmetry plane, it is
advantageous to solve the EM field problem using the integral formulation. The most renowned
of these formulations is the mutual inductance method first introduced by Kolbe and Reiss [70]
and applied to induction heating problems by Dudley and Burke [71]. In this method, the system
is divided into a elementary circuits whose volume elements possess constant current density.
The eddy currents in each circuit may be expressed in terms of the contributions of all other
circuits in the system, and the resulting set of simultaneous equations are solved to yield the
current distribution. Relations for calculating the self-inductance and mutual inductance may be
easily found in electrical engineering textbooks [72]. Complementing this method’s simplicity is
the fact that it may be used to solve the EM field problem in multiply-connected arbitrary
domains without having to grid free space. This method has been applied to modeling material
processing systems such as induction furnaces [21, 25, 26, 30, 73], the continuous casting of
aluminum [3, 74], and levitation melting systems [75].
2.2—Modeling of Heat Transfer during Solidification
Solidification is a classical moving boundary problem which involves the transfer of heat
and mass. Development of mathematical modeling tools to describe solidification processes
12
involving the solution of the heat, mass and momentum transfer equations is of paramount
importance in order to understand and predict solidification phenomena.
Initial efforts to develop a mathematical description of solidification processes were
focused on idealized problems assuming no convection in the liquid phases (i.e. stagnant liquid)
and pure materials. Such studies were later expanded to include alloy systems.
2.2.1—Isothermal Solidification
Solidification of pure metals or other materials which undergo isothermal phase change
(e.g. eutectic alloys), constitute a well-known class of moving boundary problems known as
Stefan problems. The solution of these problems requires determining the temperature profile in
each phase via the solution of the heat conservation equations for both the solid and liquid,
respectively, followed by foreknowledge of the rate of solidification front advancement in order
to resolve the Stefan conditions at the interface.
The earliest solutions of one dimensional Stefan problems were exact analytical in nature
for a semi-infinite medium by employing a similarity solution technique, transforming the partial
differential equations into ordinary ones. Such an approach is necessary due to the non-linear
nature of the energy balance at the interface. Those interested in the mechanics of these solutions
may refer to the heat transfer text of Eckert and Drake [76]. In order to obtain such solutions,
however, numerous assumptions and simplifications are required; this limits their applicability
with regards to bounded systems. To this, approximate integral methods were developed for
specific bounded systems by Goodman [77], Lightfoot [78], Rathjen and Jiji [79], and Budhia
and Krieth [80]. However, these methods still require a number of simplifications, and thus will
13
not be discussed further in the context of this work. For more information on solution of Stefan
problems, see the text of Rubenstein [81].
The limitations of the previously mentioned analytical methods led to the development of
numerical solutions of Stefan problems in multiple space coordinates. Since isothermal phase
change materials feature a sharp, distinct interface, there is a likewise strong discontinuity. This
discontinuity may be treated with the use of front-tracking, boundary immobilization, or specific
heat methods.
Murray and Landis [82] were the first to introduce the front-tracking approach. In this
solution method, the grid features a set of zero dimensional marker nodes to explicitly define the
interface location, and are connected using a piecewise function—typically a polynomial. While
the grids located at a distance from the moving boundary are fixed and regular in shape, those
nearest the interface are deformed and irregular in shape. In the work of Unverdi and Tryggvason
[83], an indicator function was used to define the interface by assigning integer values to each
phase. The marker nodes were then defined using an interpolant based off the interfacial energy
balance, and the nodes were allowed to propagate through the fixed grid. However, this method
cannot easily handle three dimensional solidification. This led to the level set method of Osher
and Sethian [84], which relies on the determination of a level set function that satisfies the
Hamilton-Jacobi equation. The interface is defined as the zero level set. Implementation is
computationally expensive, however, due to the method requiring a very fine grid structure near
the interface.
Boundary immobilization methods solve the governing heat equation by transforming
each single phase domain from real space to a non-orthogonal computational space. The
interface in this new system lies on a single, fixed coordinate surface with mobile outer
14
boundaries, making the solution method Lagrangian in form. This method was first employed for
one dimensional interfaces by Crank [85] and later extended to two dimensions by Duda et al
[86] for phase change of a finite bounded cylinder. In Saitoh [87], the system was mapped using
the Landau transformation, which reduces the number of space variables by one. Each of the
previous studies used the finite difference method to achieve a solution, while Hsu et al [88] used
the control volume method to solve the transformed equations. Although boundary
immobilization has been shown to produce accurate solutions to benchmark problems, the
transformed equations contain nonlinear cross-derivative terms consisting of multiple spatial
derivatives, making implementation cumbersome.
The specific heat method, first introduced by Thionov and Samarskii [89], avoids the
need to explicitly discretize the boundary by introducing an effective specific heat capacity in the
neighborhood of the transformation temperature by assuming that the discontinuity in enthalpy
can be represented by an extremely narrow freezing range. This allows the latent heat term in the
heat conservation equation to be rewritten in terms of a piecewise specific heat function. A
thorough introduction of the method may be found in Szekely and Themelis [90]. The first
applications of the specific heat method is found in Soviet literature [91, 92]. For materials
which undergo isothermal phase change, the specific heat function for latent heat release was
assumed to be linear with temperature.
2.2.2—Solidification of Alloys
Unlike pure materials, most alloys do not undergo isothermal phase change; instead, the
transition from the liquid to solid phase occurs over a temperature range. Alloy solidification
begins at liquidus temperature, and concludes at the solidus temperature. Due to the incremental
15
nature of the phase change, front tracking and boundary immobilization algorithms are not
applicable to modeling alloy solidification at the macroscale.
Latent heat evolution during alloy solidification is determined by the transformation
kinetics. Models representing this evolution may be divided into two categories, namely
empirical and deterministic formulations. In empirical models, the fraction solid is given as a
continuous function of temperature. There are a number of functions available to represent the
fraction solid. The simplest is that where the fraction solid is given as a linear function of
temperature, as seen in the works of Voller and Prakash [32], Chang and Stefanescu [93] and
Poole et al [6], among others. Other relations that have been used is the lever rule used by
Incropera and colleagues [33, 38], and the Scheil relation used by Santos et al [94]. However,
empirical models do not include any information regarding the microstructural features of the
crystallites in the mushy region. First proposed by Oldfield [95], deterministic models determine
the value of solid fraction via nucleation and growth laws rather than temperature dependent
functions. The heat evolved is then given by the change in volume of the growing nuclei and
crystallites. This approach was then applied by Stefanescu and colleagues [96, 97] for predicting
the cooling curves of cast iron and by Budenkova et al [98] and Wu et al [99] for solidification of
Al-Si alloys.
2.3—Modeling of Fluid Flow during Solidification
Early models for solidification assumed that the molten material was quiescent, making
the convective derivatives zero, for the sake of simplifying the solidification problem.
Experimental observations, however, have shown that this assumption is quite rare, and the
presence of fluid flow and convective heat and mass transfer leads to significant deviation from
16
diffusion-only solutions. Such phenomena have been shown to have a strong influence on
microstructural development and segregation profiles of the final cast product [10-21].
There are two fundamental regimes of convective transport during solidification: (i)
natural convection and forced convection. In natural convection, also referred to as thermosolutal
convection, fluid flow occurs as a result of thermal and solute gradients in the liquid phase. The
relative intensity of natural convection in the system is defined by the Rayleigh number, which is
the ratio between the buoyancy and viscous forces. Theoretical studies [100, 101] found that the
critical value of the Rayleigh number for the onset of natural convection in alloys to be ~10 4 .
Experiments involving aqueous alloys have shown that fluid flow causes alterations in
the solidification velocity and curvature of the melt front [102, 103], which are both important in
determining the solidification morphology and grain size [104]. Furthermore, macrosegregation
is directly caused by transport of rejected solute via interdendritic and bulk flow throughout the
solidifying cast alloy [105].
Forced convection, however, occurs via applied body forces originating from an external
source. These forces may be based on mechanical [106], ultrasonic [107], or electromagnetic
phenomena. The effects of forced convection on the micro- and macrostructure have been well-
documented. Liu et al [12] found that forced convection homogenized the alloying elements in
the AZ91 melt, and also improved solution strengthening of the alloy. Kuznetzov [108] found
considerable inverse macrosegregation of carbon in twin-rolled cast steels. However, the most
important role of stirring is that of grain refinement via the dendrite fragmentation mechanism,
as this increases the nucleation potential of the melt [19-21].
While much focus has been dedicated to understanding the flow in the bulk liquid in
metalcasting systems, convection, regardless of source, is also found in the mushy region as well
17
[109, 110]. There have been several formulations proposed in order to understand the flow in
these two domains. Such formulations may be succinctly characterized as either (i) single-zone
or (ii) dual zone models.
2.3.1—Single Zone Models
In single-zone formulations, the dendrites are assumed fixed in place for all values of
fraction solid greater than zero, and thus may be treated as a porous medium that obeys Darcy’s
law. The permeability decreases with increasing fraction solid, leading to increased damping of
the flow as solidification progresses. The first model was that introduced by Mehrabian et al
[111] to describe the role of interdendritic flow on solute redistribution, but the solution domain
was restricted to the mushy region only. Szekely and Jassal [112] later expanded the model to
include the contributions of the bulk liquid flow on solute redistribution.
The permeability relations are expressed in terms of the geometry of the crystallites in the
porous medium and their respective instantaneous grain size. The geometrical dependence of the
permeability means that there may exist a high degree of anisotropy depending on the
directionality of the flow, making the permeability a tensor of second order. However, for
macroscale modeling of equiaxed solidification, the orientations of the crystallites in the control
volume are assumed to be random, leading to the geometrical dependence of the permeability to
be taken as isotropic. A number of permeability models have been used in modeling
solidification systems. The Hagen-Poiseuille model describes the permeability assuming laminar
flow through a bundle of tubes [31, 36, 111].This is a good approximation for columnar
solidification, and was primarily used in studies by Mehrabian and coworkers [31, 111]. In the
case of equiaxed and globular morphologies, the permeability is given by the Kozeny equation
18
and its derivatives [35, 113], which assume laminar flow through an array of packed spheres.
Use of the Kozeny relationships may be found in Voller and Prakash [32], Incropera [33, 38],
and Campanella [34] among others. It should be noted that other analyses have been performed
to adjust the permeability relations to account for the tortuosity of dendritic morphological
structures [114].
It should be noted that the assumptions used for single-zone models, particularly the
permeability relations, are valid for laminar flow only; however, there have been attempts to
account for turbulence in the mushy region. Shyy et al [37, 115] was the first to incorporate
turbulence in single-zone models. The model accounted for damping of turbulence using a low
Reynolds number k-ε model. However, the Shyy formulation only assigned an ad-hoc functional
dependence to the turbulence constant Cμ, leaving the constants associated with turbulent
generation unaltered and thus preventing closure of the k and ε equations. Prescott and Incropera
[38] represented the first attempt to describe turbulent flow in EM solidification systems. The
model used the low-Re k-ε of Jones and Launder [116]. Although turbulent closure was attained
and reported significant damping of turbulence in the mushy region, the formulation
incorporated Darcy-like terms into the k and ε equations. Such relations do not reflect the
physics of the problem for two reasons, as (i) Darcy’s law only applies to laminar flow and (ii)
the turbulent mixing length within the interdendritic region quickly become on the order of the
Kolmogorov length scale, making the flow essentially laminar with regards to macroscale flows
[117].
19
Although single-zone models have proven useful in describing interdendritic flow for
castings exhibiting columnar grain structures, experimental investigations [109, 110] have found
the porous medium assumption to be wholly inadequate for equiaxed solidification, where the
crystallites travel with the liquid and form a slurry. It was also found that Darcy behavior only
occurs at higher solid fraction [109, 110].
This presents the impetus for a new model to account for the varying behavior of the
crystallites with respect to fraction solid. The first attempt was made by West [118], which used
a piecewise function for the permeability function. This was used by Amberg [119] for
macrosegregation of steel. Although this addresses the dualistic behavior of equiaxed crystallites
in the mushy region, the model still does not account for the dynamic behavior of the crystallites
at low fraction solid. Furthermore, for reasons previously mentioned, the West model may not be
applied to turbulent flow regimes.
Oldenburg and Spera [39] accounted for the traveling crystallites by relaxing the packed
bed assumption at low fraction solid and splitting the mushy region into two flow domains,
shown in Figure 2-1. In the suspended particle region, the liquid and crystallites were treated in
aggregate as a slurry. The flow in this region was treated as that of a “pseudofluid” using the
homogeneous flow model, with the viscosity having dilatant behavior. The porous medium
relation was retained for the fixed particle region. The two domains were separated using the
coherency fraction solid, whereby the crystallites begin to come into contact with one another
and form an interlocking mesh. This approach was applied by Chang and Stefanescu [93] and
Mat and Ilegbusi [120] in modeling shrinkage-driven macrosegregation in metal alloys and
aqueous analogues.
While the Oldenburg and Spera formulation accurately reflects the physical phenomena
associated with equiaxed solidification, the original formulation is limited to laminar flow;
however, forced convective flows are typically highly turbulent [3, 21, 50]. Pardeshi et al [42]
recently presented a dual-zone formulation that accounts for turbulent behavior by using the
high-Re k-ε model of Launder and Spalding [121] throughout the bulk liquid and the mushy
region. However, use of this model in the fixed particle region leads to the same mixing length
pitfalls as was found for Prescott [38] and Shyy [37,115], making closure unattainable.
However, the greatest drawback of the Pardeshi model lies in the lack of accounting for
momentum damping in the suspended particle region. It was shown as early as Brinkman [122]
that there is an additional friction force exerted by the solid phase in the turbulent particle flows,
with a similar results being found by Saffman [123] and Sproull [124]. In his study on ice slurry
flows, Shire et al [125] noted that the phenomenon of “re-laminarization” was more prominent at
higher values of ice fraction, and theorized that it was due to the slurry preventing the generation
of turbulence. Yamagishi et al [126] further elaborated on re-laminarization, attributing it to the
turbulent mixing length becoming on the same order as the particle size. For further instances of
laminarization in initially turbulent slurry flows, the reader is also referred to the studies of
Wenji et al [127] and Alvarado et al [128]. It should be noted that Budenkova et al [98] made
attempts to account for the interactions between the crystallites and the turbulent eddies using a
damping function. While turbulence was damped, the expressions used were ad-hoc in form and
lacked any physical foundation.
The redistribution of solute at the solid-liquid interface induces spatial variations in the
concentration of alloying elements within the casting, commonly referred to as segregation. Such
variations are deleterious to ensuring uniform physical properties within the cast alloy, and thus
should be minimized. Solute segregation phenomena may be divided into microsegregation and
macrosegregation. Microsegregation takes place at the interface due to differences between the
solute solubility in the different phases, while macrosegregation takes place due to the bulk
transport of solute enriched (or depleted) liquid throughout the casting. It should be noted that
macrosegregation is present even in the absence of stirring forces.
Since the focus of this work is macroscale modeling, only macrosegregation will be
discussed. The first macrosegregation models were developed by Kirkaldy and Youdelis [129],
Flemings and Nereo [130], and Mehrabian et al [111]. These models were applied to shrinkage-
driven and buoyancy-driven flows, and are able to predict the occurrence of inverse segregation
in cast Al-Cu alloys. However, these models are applicable to flow in the mushy region only and
cannot be used for forced convective flows.
The first model to include the effects of bulk liquid flow on macrosegregation was that of
Ridder et al [31]. In this formulation, the solidifying domain was divided into the mushy and
bulk liquid regions (i.e. single-zone model). The shrinkage-induced flow field was calculated
from Darcy’s law. The flow in the bulk liquid was determined via stream function solutions, and
the two flow fields were resolved using pressure-based boundary conditions applied at the
liquidus isotherm. The solute field was then calculated using the local solute redistribution
equation of Flemings and Nereo [130]. Although the Ridder model does accurately predict
segregation profiles found in Pb-Sn castings; however, the domain decomposition method
22
employed can only be used for steady state problems, as the conforming mesh used to obtain a
solution relies on the foreknowledge of the liquidus isotherm position.
The development of continuum models in the eighties allowed for the description of
solute transport in both the bulk liquid and mushy regions. First introduced by Bennon and
Incopera [33] and Voller and Prakash [32], such models using mixture theory in defining the
solute concentration within a given control volume, whereby the conservation equations in each
phase are summed with respect to the relative presence of each phase within the control volume.
The thermophysical properties (e.g. mass diffusivity) of the mixture are similarly treated. Such
approaches allow for a simplified solution of the resulting equations for fixed grids without
explicitly having to define interface locations.
The coupling of the micro-scale segregation phenomena with continuum formulations is
necessary to determine the rate of solute rejection into the surrounding liquid. The simplest
method of coupling is through assuming the diffusional behavior of solute in each phase. Early
continuum models such as that of Bennon and Incropera [33] assumed complete diffusion within
each phase and, by corollary, compositional homogeneity within each phase. The lever rule, as it
is often referred, has been applied in a clear majority of macrosegregation studies, examples of
which may be found in References [33, 42, 131, 132]. However, the assumption of significant
solid state diffusion is not physically valid, as the value of mass diffusivity in the solid to be
several orders of magnitude smaller than that of the liquid.
Recognizing this, Rappaz and Voller [133] proposed an alternative approach by assuming
no diffusion within the solid phase while maintaining complete diffusion in the liquid (aka Schiel
assumption). This allows for the elimination of solid diffusion terms within the overall
conservation equation and, by assuming equilibrium conditions at the solid-liquid interface,
23
allows for the determination of the overall solute balance while only solving for the liquid
concentration only. This method was applied in the study of inverse segregation of Al-Cu alloy
by Chang and Stefanescu [93] using a dual-zone flow model, and was found to be in good
agreement with measurements; the model was also employed by Barman and Dutta [47]. There
have also been efforts to incorporate a finite amount of solid state diffusion into the solidification
model, as reflected later formulations by Voller and colleagues [134-136]. However, as noted in
the vanguard work [133], the principal drawback of this model lies in its use of the interfacial
equilibrium assumption. While it may be used for solidification problems, it may not be applied
in reverse; that is, the assumption is invalid for remelting problems unless the freezing history is
known.
24
Chapter 3
An Improved Model for the Flow in an Electromagnetically Stirred Melt during Solidification
3.1—Abstract
A mathematical model for simulating the electromagnetic field and the evolution of the
temperature and velocity fields during solidification of a molten metal subjected to a time-
varying magnetic field is described. The model is based on the dual suspended particle and fixed
particle region representation of the mushy zone. The key feature of the model is that it accounts
for turbulent interactions with the solidified crystallites in the suspended particle region. An
expression is presented for describing the turbulent damping force in terms of the turbulent
kinetic energy, solid fraction, and final grain size. Calculations were performed for solidification
of an electromagnetically stirred melt in a bottom chill mold. It was found that the damping force
plays an important role in attenuating the intensity of both the flow and turbulent fields at the
beginning of solidification, and strongly depends on the final grain size. It was also found that
turbulence drops significantly near the solidification front, and the flow becomes laminarized for
solid fraction around 0.3.
Electromagnetic (EM) stirring has found extensive use in solidification processing as a
means to produce a fine, equiaxed grain structure [1-3]. The role of the flow is to homogenize
the solute and temperature profiles in the bulk liquid [4,5], which affects segregation in the cast
product. It also increases the nucleation potential in the melt through a combination of dendrite
fragmentation [6-8], a decrease of the temperature gradient at the solidification front [9], and an
25
increase the dissipation rate of the melt superheat [10]. Clearly, an improved understanding of
the flow characteristics in the bulk and mushy zones during solidification is critical in order to
control the structure of the final product.
There are essentially two basic approaches for modeling the flow in the mushy zone,
namely single-zone [11] and dual-zone models [12]. The single-zone model treats the entire two-
phase region as a porous medium, with the flow being damped via Darcy’s law. Although this
model provides an adequate representation of the flow in columnar solidification, it is not
suitable for equiaxed solidification, as the crystallites have been shown to travel with the flow
prior to coalescence [13].The dual-zone model addresses this problem by dividing the mushy
zone into two domains: (i) the suspended particle region, and (ii) the fixed particle region, with
the transition between regions occurring at the coherency point.
Recently, efforts have been made to model EM solidification processes [14-21]. With no
exception, all models used an approximate analytical solution for describing the EM force field
in the bulk liquid and two phase regions. In modeling the flow in the mushy zone, all of these
studies, except for the works of Pardeshi et al [20] and Budenkova et al [21], employed a single-
zone model for describing fluid flow in the mushy region. Several approaches have been used to
model the turbulent field in the two phase region. Prescott and Incropera [15,16] and Shyy et al
[17,18] determined the turbulent field using a low-Re k-ε model, together with ad-hoc
expressions for the decay of the turbulent viscosity in the two phase region. Pardeshi et al [20]
and Budenkova et al [21] employed high-Re k-ε model to describe the turbulent characteristics in
the bulk liquid and suspended particle regions. Their formulation does not account for the
damping of turbulence in both the suspended and fixed particle regions. Furthermore, the
26
interaction between the turbulent eddies and the solid crystallites, which is known to produce an
additional damping force on the flow field [22-24], was not addressed in these models.
This paper presents a comprehensive model for the numerical calculation of the
electromagnetic, velocity and temperature fields in an axisymmetrical EM stirred melt during
solidification. This model uses a dual-zone approach for the flow in the mushy zone, and
accounts for the damping of turbulence using the low-Re k-ε model, along with a turbulent
damping force resulting from the interactions between the turbulent eddies and the crystallites in
the suspended particle region. The model is then demonstrated for unidirectional solidification in
a bottom-chill mold stirred using an induction coil.
3.3—Model Formulation
Figure 3.1—Sketch of a typical EM stirred solidification system
Figure 3.1 shows a typical EM stirred solidification system. As seen in this figure, the
system is comprised of a container and heat extraction devices, surrounded by induction coil. An
electric current is passed through the coil to induce eddy currents in the metal. The induced
27
currents generate both heat via electrical energy dissipation and Lorentz forces, which drive the
flow in the bulk liquid and mushy zones. Numerical simulation of the solidification process must
involve calculation of the EM field in the metal and other conducting domains, the velocity and
turbulent fields, and the temperature field.
3.3.1—Electromagnetic Field
In this work, the electromagnetic field was calculated by solving the integral form of the
Maxwell equations using the mutual inductance method [25-28]. In this method, the system (the
metal and the magnetic shields) are divided into a number of elementary circuits, each of which
is considered to be a region of constant current density, J. For a time-harmonic two dimensional
field, the induced currents in the elementary circuits can be represented by the following set of
algebraic equations:
1 1 1
. metal shields coil
i i m i c i k km c m c k
d j M M M I

J l J S J S [3-1]
where j is the square root of -1, σ is the electrical conductivity, µ0 is the magnetic permeability of
free space, dl is the length of the circuit, S is the cross-sectional area of the circuit, and Mi,k is the
mutual inductance given by
l l [3-2]
From the induced current, the magnetic flux density, B, can be obtained from:
j
J B [3-3]
Finally, from the induced current and magnetic fields, the electrical energy dissipation (Joule
heating), Sem, and the Lorentz force distribution in the melt, Fem, can readily be calculated from
28
*1
where J * denotes the complex conjugate of the current density.
3.3.2—Heat Transfer
The general energy equation that describes heat transfer and solidification in the metal
domain is
t dt
u [3-6]
where ρ and L are the density and latent heat of fusion, respectively. Assuming that solid fraction
is a piecewise linear function of temperature, the latent heat term in Eq. (3-6) may be eliminated
,
*
,
c T T
[3-7]
where n corresponds to the number of segments and Ti and Ti+1 represent the temperatures
defining an individual line segment in the solid fraction versus temperature curve. TL and TS are
the liquidus and solidus temperatures, respectively, and the l and s subscripts correspond to the
values for the respective liquid or solid phases. For convective heat transfer in turbulent flows,
the effective thermal conductivity, k * , is given by
29
s S
k T T
[3-8]
where μt is the turbulent viscosity and PT is the turbulent Prandtl number.
3.3.3—Fluid Flow
Figure 3.2—Flow domains for the dual-zone solidification model
Figure 3.2 shows the various flow domains in the dual-zone model, namely the bulk
liquid, suspended particle region, and fixed particle region. In the suspended particle region, the
flow is described using the homogeneous two-phase flow model, and the flow is driven by EM
forces, as in the bulk liquid. In the present model, damping of the flow via interactions between
the turbulent eddies and the solid crystallites is considered. In the fixed particle region, the flow
is represented by Darcy’s law. It should be mentioned that the Lorentz forces do not drive the
flow in the interdendritic channels. In this work, the flow in the fixed particle region is assumed
to be laminar, which is a reasonable assumption since the interparticle spacing is on the order of
the Kolomogrov turbulent length scale [29].
30
Continuity:
where 1s s s lf f u u u [3-10]
Navier-Stokes Equation:

u u u u u F F u u [3-11]
where μ is the effective viscosity, and λ is a switch parameter, Fd is the damping force due to
turbulence interactions with the solid particles, and P is the pressure. For the suspended particle
region, u=us, making the Darcy term equal to zero, and λ is equal to unity. For the fixed particle

where Dg is the final grain size.
The turbulent field is described using the low-Re k-ε model [30]. The conservation equations for
k and ε are

u [3-14]
where Pk and Pε are the turbulent Prandtl numbers for k and ε equations, respectively, and μt is
the turbulent viscosity given by
2
In the low-Re k-ε model, the turbulence constants C1 * , C2
* , and Cμ
Reynolds number (RT=ρk 2 /μlε):

*
[3-16]
where μl is the laminar viscosity, and C1, C2, and Cμ are equal to 1.43, 1.92, and 0.09,
respectively. The effective viscosity is the sum of the laminar and turbulent viscosity
components. The laminar viscosity is determined from the rheological properties of suspensions
[31], and for each flow domain may be expressed as:
2
0
1
m c s
f f
3.3.4—Turbulent Damping Model
21 . d L tf F [3-18]
where fL is the liquid fraction, and τt is the turbulent Reynolds stress. Detailed derivation of Eq.
(3-18) is given in Appendix 3A. Following Bradshaw’s turbulent model [32], the Reynolds stress
can be written in terms of turbulent kinetic energy as:
1/2
t d ijc k [3-19]
where cd is a constant, and is equal to 0.08 [33]. Hence, the divergence of the Reynolds stress is:
32
1/2. t dc k [3-20]
The grad term in Eq. (3-20) represents the change in turbulent kinetic energy between the
surrounding liquid and the particle surface, where k is taken to be zero. For particles of
instantaneous size d arranged in a cube of dimension Dg, the grad of the turbulent kinetic energy
can be locally approximated by

k k
D d
e [3-21]
From Eqs. (3-18), (3-20), and (3-21), the damping force is given by:
1/2
[3-23]
The quantity β represents the particle-to-envelope volume ratio. The value of β for spherical
particles is unity, and decreases with increasing sphericity. In addition, β also defines the
coherency solid fraction (fc=πβ/6), which determines the boundary between the suspended
particle and fixed particle flow domains. From Equations (3-22) and (3-23), the damping force
can be written as:
F e [3-24]
3.4—Solution Technique
The heat and fluid flow equations were solved using the control volume technique of Pun
and Spalding [34]. In this technique, the solution domain was divided into a number of
33
contiguous volume elements. The momentum equations were discretized using the upwind
scheme, and the resulting equations were solved iteratively. The pressure field was calculated
using the SIMPLE algorithm of Patankar [35]. In these calculations, the solution was carried out
for a 30 x 30 grid, which is sufficient to resolve the velocity and turbulent fields in EM induction
stirring systems [27].
The magnetic field was calculated by dividing the metal and adjacent conducting regions into a
number of elementary circuits. In order to accurately describe the decay of the magnetic field in
the metal (skin effect), a finer grid was used near the outer radius of the conducting domains.
The current density in each circuit is evaluated using Eq. (3-1), and the resulting set of
simultaneous equations was solved using Choleski factorization. Upon obtaining the J field,
Ampere’s law is used to obtain the B field. From the computed J and B fields, the
electromagnetic forces and Joule heating are calculated.
3.5—Results and Discussion
In this section, we shall present the computed results for unidirectional solidification of
Al-4.5%Cu alloy in a bottom chill mold surrounded by an induction coil. The induction coil
employed in this study consists of three turns situated in the middle of the crucible. The mold is
comprised of an insulating refractory tube and a water-cooled stainless steel chill block. The
dimensions of the system are given in Figure 3.3. Calculations were carried out for a coil current
and frequency of 200 A and 500 Hz, respectively, a coherency solid fraction of 0.521, which
corresponds to a globular solidification morphology, and the final grain size of the cast alloy, Dg,
varying from 100 to 500 m. The thermophysical properties used in this study are given in
Table 3.1.
Figure 3.3—Dimensions of the system used in this study
Solid density: 2979 kg/m 3
Liquid density: 2979 kg/m 3
Solid thermal conductivity: 188.3 W/m-K
Liquid thermal conductivity: 192.5 W/m-K
Solid heat capacity: 870.5 J/kg-K
Liquid heat capacity: 1059 J/kg-K
Electrical conductivity: 1.28*10 6 Mho/m
Liquidus temperature: 921 K (648°C)
Solidus temperature: 837 K (564°C)
Latent heat of fusion: 389000 J/kg
Molecular viscosity: 0.0015 Pa-s
Heat Transfer Coefficient 500 W/m 2 -K
Table 3.1—Thermophysical properties of Al-4.5%Cu alloy
Figure 3.4 shows the computed EM force field in the metal and the chill block. As seen in
this figure, the EM force is at a maximum in the middle of the metal where the coil is located. It
is also seen that the EM forces in the chill block are much smaller than those in the metal. Closer
inspection of this figure shows that the EM forces near the chill block are higher than those at the
top of the melt. This suggests that the vorticity of the EM forces, which drives the flow, will be
asymmetrical, as shown in Figure 3.5. This figure also shows two counter-rotating vortices,
35
which suggests of two recirculating flow loops typical for a stationary magnetic field. The
difference in the spatial variation of the vorticity, however, suggests that the intensity of the flow
in each loop will be different. The distortion of the force field by the chill block underscores the
necessity of including numerical computation of the electromagnetic field for simulating EM
stirring processes.
Figure 3.4—Computed Lorentz (EM) force field in the metal and chill block
36
Figure 3.5—Computed vorticity of the EM force field in the metal
Figure 3.6 shows the initial velocity and turbulent fields of the flow prior to
solidification. The turbulent field is represented in terms of the ratio of the turbulent to laminar
viscosities, μ * . As seen in Figure 3.6(a), the flow consists of two axisymmetric recirculating
loops, consistent with the computed curl of the EM force field, Figure 3.5. For the given coil
current and frequency, the characteristic velocity is around 25 mm/s. Closer inspection of this
figure shows that the flow intensity in the upper loop is stronger than the lower loop. The
maximum velocity in the upper loop is about 32 mm/s, while it is around 27 mm/s in the lower
loop. Figure 3.6(b) shows that the turbulent viscosity is quite high, around 50 times the laminar
viscosity of the liquid. It also shows that there is a significant spatial variation in the values of
the turbulent viscosity, with the largest values found at the center of the vortices and at the free
surface, where the shear strain rates are highest.
37
Figure 3.6—Initial characteristics of the flow: (a) velocity and (b) turbulent-to-laminar
viscosity ratio
Figures 3.7(a) through 3.7(d) show the evolution of the velocity field during solidification
at times of 30, 60, 120, and 240s, respectively. These results correspond to a final grain size of
500 µm. When solid fraction is less than 0.05, Figure 3.7(a), the velocity field is essentially the
same as that prior to solidification and the characteristic velocity is around 22 mm/s. After 60s,
Figure 7(b), there is some reduction in the flow intensity. This is particularly more noticeable in
the lower loop, where solid fraction is around 0.15. The characteristic velocity of the flow in this
region is about 15 mm/s.
38
Figure 3.7—Computed velocity profiles in the metal at: (a) 30s, (b) 60s, (c) 120s, (d) 240s.
Contours correspond to values of solid fraction.
39
Fig. 3.7(c) shows that damping of the flow is noticeable when solid fraction becomes
greater than 0.25, with a characteristic velocity of 10 mm/s. The differences between the flow in
the fixed particle region and the suspended particle region are clearly illustrated in Figure 3.7(d),
which shows the flow characteristics after 240s. As seen in this figure, the flow in the fixed
particle region is almost negligible compared with that of the suspended particle region. The
velocity at the edge of the fixed/suspended particle regions is about 2 mm/s, and drops to 0.1
mm/s with increasing solid fraction. These results suggest that the velocity in the suspended
particle region is quite large for EM stirred systems and cannot be ignored when describing heat
and mass transfer phenomena. It should also be mentioned that this finding is a corollary to those
reported by Oldenburg and Spera for strong thermosolutal convection in the mushy zone during
solidification [12].
Figures 3.8(a) through 3.8(d) show the corresponding evolution of the turbulent field
during solidification. At the beginning of solidification, Fig. 3.8(a), there is a marginal drop in
the turbulent viscosity, particularly in the lower loop where solidification was initiated. The drop
in the viscosity is more pronounced when the solid fraction is between 0.1 and 0.15, Fig. 3.8(b).
Fig. 8(c) shows that turbulence is effectively damped after 120s, where solid fraction is around
0.3. The flow is completely laminarized as solid fraction approaches the coherency value, Fig.
3.8(d). It is interesting to see that the decay of turbulence occurs more rapidly than that of the
velocity. This is expected, as the turbulent energy generation rate is proportional to the square of
the velocity.
(a) 30s, (b) 60s, (c) 120s, (d) 240s
41
It is instructive to compare the results of the presented model, which accounts for
turbulent damping, with those which do not include such damping for EM stirred systems
[20,21]. Figure 3.9 shows the variation of the velocity in the suspended particle region with
respect to solid fraction. The values presented here have been normalized with respect to the
velocity at zero solid fraction (v*=v/v0). This figure shows that ignoring the damping force does
not lead to any change in the velocity until solid fraction is above 0.45. It should be mentioned
that the sudden drop of the velocity near the coherency point is due to viscous effects at the
boundary layer of the porous wall. This finding is particular to forced convection systems, where
the external forces are relatively unaltered in the suspended particle region.
Figure 3.9—Comparison between the velocity in the suspended particle region
with and without damping force
Figure 3.10 shows the variation of the turbulent viscosity versus solid fraction in the
suspended particle region. This figure shows that the damping force causes the turbulent
viscosity to decrease linearly with solid fraction across the suspended particle region. These
results suggest that neglecting these interactions could lead to errors in computing the velocity
42
and turbulence levels in the mushy region, which could have profound effects on predicting
solute segregation.
Figure 3.10—Comparison of turbulence in the suspended particle region
with and without damping force
Figure 3.11—Influence of final grain size, Dg, on damping of velocity in the
suspended particle region
43
Figure 3.12—Influence of final grain size, Dg, on damping of turbulence in the
suspended particle region
Since the damping force depends on the final grain size, it is interesting to examine its
effect on the flow in the mushy zone. Figure 3.11 shows the variation of the velocity in terms of
solid fraction for final grain sizes of 100, 200, and 500µm. As seen in this figure, the velocity in
the suspended particle region decays more rapidly for decreasing grain size. Figure 3.12 shows
the corresponding variation of the turbulent viscosity as function of solid fraction in the
suspended particle region. It should be noted that the decrease of the turbulent viscosity is faster
than the velocity. These results suggest that the flow characteristics in the two-phase zone
critically depend on both the solidification rate and nucleation potential of the melt, which
dictate the grain size [36,37].
3.6—Conclusions
In this paper, an improved mathematical model has been presented for simulating
electromagnetic, fluid flow, and heat transfer phenomena during solidification in an EM stirred
system. The model allows for computation of the EM force field for any given coil
44
configuration, coil current, and coil frequency, and allows for the presence of magnetic shields.
The solidification model is an extension of the dual-zone formulation to turbulent flows, and
accounts for turbulent damping in the suspended particle region. An expression is presented
describing the damping force in terms of turbulent kinetic energy, solid fraction, and final grain
size.
This model was used to numerically investigate the electromagnetic field and evolution
of the temperature and velocity fields to solidification in a bottom chill mold surrounded by an
induction coil. The principal findings of this work are summarized as follows:
The magnetic shields caused significant distortions in the EM force field near the base of
the metal. This distortion affected the vorticity of the force field, which drives the flow.
Such an effect necessitates numerical solution of the EM field.
For melt stirring using a stationary magnetic field, the flow consisted of two
axisymmetric, recirculating loops, and is highly turbulent. Solidification causes
significant decay of the velocity and turbulent fields. The velocity decreases by one order
of magnitude in the suspended particle region. Laminarization of the flow occurs in the
middle of the suspended particle region for solid fraction around 0.3.
The developed expression shows that the turbulent damping force depends on the final
grain size. For smaller grains, the drop in the velocity occurs more rapidly with solid
fraction.
Neglecting the turbulent damping force led to a severe overestimation of both the
velocity and turbulence levels in the suspended particle region.
45
The paper presented here represents a more comprehensive model for EM solidification
processes. It allows for the calculation of the electromagnetic field to permit a more realistic
description of the flow in the solidification system. It also provides a model for describing
turbulent flow behavior in the mushy region. These improvements to existing models offer a
framework for better understanding the roles of fluid flow and heat transfer phenomena on
solidification in both EM stirring and other forced convection systems.
3.7—Acknowledgement
The authors graciously thank the National Science Foundation for their funding of this
project under grant CMMI-0856320.
3.8—References
[1] A.A. Tzavaras and H.D. Brody: J. Met., 1984, vol. 36, no. 3, pp. 31-37.
[2] C. Vives: in Magnetohydrodynamics in Process Metallurgy, eds. J. Szekely, J.W. Evans, K.
Blazek, and N. El-Kaddah, pp. 169-174, TMS, Warrendale, PA, 1991.
[3] Y.A. Kompan, I. Protokovilov, Y. Fautrelle, Y.U. Gelfgat, and A. Bojarevics: in Modelling
for Materials Processing, pp. 85-90, University of Latvia Press, Riga, 2010.
[4] C. Vives and C. Perry: Int. J. Heat Mass Transfer, 1986, vol. 29, pp. 21-33.
[5] Q. Zhao, X. Zhang, C. Feng, N. Zhang, Y. Han, J. Guo, and X. Hou: Adv. Mater. Res., 2012,
vols. 482-484, pp. 1447-1452.
[6] K.A. Jackson, J.D. Hunt, and D.R. Uhlmann: Trans TMS-AIME, 1966, vol. 236, pp. 149-158.
[7] B. Willers, S. Eckert, U. Michel, I. Haase, G. Zouhar: Mater. Sci. Eng. A, 2005, vol. 402, pp.
55-65.
[8] J.A. Dantzig and M. Rappaz: Solidification, pp. 464-466, EPFL Press, Lausanne, 2009.
[9] B. Wang, Y. Yang, and W. Tang: Trans. Nonferrous Met. Soc. China, 2008, vol. 18, pp. 536-
540.
[10] B. Chalmers: J. Aust. Inst. Met., 1963, vol. 8, pp. 255-263.
46
[11] R. Mehrabian, M. Keane, and M.C. Flemings: Metall. Trans., 1970, vol. 1, pp. 455-464.
[12] C.M. Oldenburg and F.J. Spera: Numer. Heat Transfer, Part B, 1992, vol. 21, pp. 217-229.
[13] C.J. Parides, R.N. Smith, and M.E. Glicksman: Metall. Trans. A, 1997, vol. 28, pp. 875-883.
[14] T. Campanella, C. Charbon, and M. Rappaz: Scr. Mater., 2003, vol. 49, pp. 1029-1034.
[15] P.J. Prescott and F.P. Incropera: J. Heat Transf., 1995, vol. 117, pp. 716-724.
[16] P.J. Prescott and F.P. Incropera: J. Heat Transf., 1993, vol. 115, 302-310.
[17] W. Shyy, Y. Pang, G. Hunter, D.Y. Wei, and M.H. Chen: Intl. J. Heat Mass Transf., 1992,
vol. 35, 1229-1245.
[18] W. Shyy, Y. Pang, G. Hunter, D.Y. Wei, and M.H. Chen: ASME J. Eng. Mater. Technol.,
1993, vol. 115, 8-16.
[19] R. Lantzsch, V Galindo, I. Grants, C. Zhang, O. Paetzold, G. Gerbeth, and M. Stelter: J.
Crystal Growth, 2007, vol. 305, 249-256.
[20] R. Pardeshi, A.K. Singh, and P. Dutta: Numer. Heat Transfer, Part A, 2008, vol. 55, pp. 42-
57.
[21] O. Budenkova, F. Baltaretu, J. Kovács, A. Roósz, A. Rónaföldi, A.M. Bianchi, and Y.
Fautrelle: IOP Conf. Ser.: Mater. Sci. Eng., 2012, vol. 33, 012046.
[22] Y. Yamagishi, H. Takeuchi, A.T. Pyatenko, and N. Kayukawa: AIChE J., 1999, vol. 45, pp.
696-707.
[23] J.L. Alvarado, C. Marsh, C. Sohn, G. Phetteplace, and T. Newell: Int. J. Heat Mass
Transfer, 2007, vol. 50, pp. 1938-1952.
[24] S. Wenji, X. Rui, H. Chong, H. Shihui, D. Kaijun, and F. Ziping: Int. J. Refrig., 2009, vol.
32, pp. 1801-1807.
[25] E. Kolbe and W. Reiss: Wiss. Z. der TH Ilmenau, 1963, vol. 9, 311-317.
[26] R.F. Dudley and P.E. Burke: IEEE Trans. Indu. Appl., 1972, vol. 8, 565-571.
[27] N. El-Kaddah and J. Szekely: J. Fluid Mech., 1983, vol. 133, 37-46.
[28] J.L. Meyer, N. El-Kaddah, J. Szekely, C. Vives, and R. Ricou: Metall. Trans. B, 1987, vol.
18, 529-538.
[29] H. Tennekes and J.L. Lumley: A First Course in Turbulence, pp. 19-20, MIT Press,
Cambridge, 1972.
[30] W. P. Jones and B.E. Launder: Int. J. Heat Mass Transfer, 1972, vol. 15, pp. 301-314.
47
[31] D.G. Thomas: J. Colloid Sci., 1965, vol. 20, pp. 267-277.
[32] P. Bradshaw, D.H. Ferriss, and N.P. Atwell: J. Fluid Mech., 1967, vol. 28, pp. 593-616.
[33] B.E. Launder and D.B. Spalding: Mathematical Models of Turbulence, p. 78, Academic
Press, London, 1972.
[34] W.M. Pun and D.B. Spalding: Report HTS/76/2, Imperial College of Science and
Technology, London, August 1977.
[35] S.V. Patankar: Numerical Heat Transfer and Fluid Flow, Hemisphere Publishing, New
York, 1980.
[36] G. Poole, N. Rimkus, A. Murphy, P. Boehmcke, and N. El-Kaddah: in Magnesium
Technology 2012, eds. S.N. Mathaduhu, W.H. Sillekens, N.R. Neelmeggham, and N. Hort, pp.
161-164, Wiley, New York, 2012.
[37] L. Nastac and N. El-Kaddah: IOP Conf. Ser.: Mater. Sci. Eng., 2012, vol. 33, 012084.
48
Appendix 3A—The Damping Force in the Suspended Particle Region
In the suspended particle region, the fluctuating velocity of the solid particles is zero, and the
instantaneous velocity of the two-phase mixture is
'' L L L s sf f u u u u u u [A3-1]

'
' '
s s L L L s s L L L
l s s L L L em
f f
u u u F

u uu u F [A3-3]
where τt is the Reynolds stress tensor. From Eqs. (3-11) and (A3-3), the damping force is given
by
49
Chapter 4
The Effect of Coil Design on the Temperature and Velocity Fields during Solidification in
Electromagnetic Stirring Processes
4.1—Abstract
This paper examines the role of induction coil design on stirring of molten metal in
electromagnetic (EM) solidification processes. A model is presented to describe the EM, heat
transfer, and fluid flow phenomena in these processes. It is based on a dual-zone description of
the mushy region, and accounts for damping of turbulence by the solidified crystallites. The
electromagnetic field equations were solved using the mutual inductance technique, while the
temperature and turbulent flow fields were calculated using the control volume method.
Calculations were performed for solidification of an Al-Cu alloy placed in a stationary magnetic
field generated by an induction coil. The effect of coil design on the flow structure was
investigated for three different coil positions. It was found that changing the coil position
significantly alters the flow pattern from four recirculating loops when the coil is above the
midsection of the melt to two loops, typical of a travelling magnetic field, when the coil is at the
base of the melt. This significantly modifies the rate of solidification across the ingot, as well as
the temperature gradient, in the mushy region. The decay of the velocity and turbulent fields in
the mushy region was found to be exponential, with the maximum rate of decay at the
solidification front. These results indicate that through changes in coil design, it is possible to
control the flow characteristics and solidification behavior in the molten metal.
50
Electromagnetic stirring technologies have found extensive use in solidification
processing of metals as a means to produce castings exhibiting fine-grained equiaxed structure.
The flow serves to minimize thermal gradients in the molten pool 1)
and rapidly dissipates the
, which in turn promotes an early occurrence of the columnar-to-equiaxed
transition 3,4)
. In addition, it increases fragmentation of the secondary dendrite arms, leading to a
higher nucleation potential in the melt 1,5,6)
. Clearly, understanding flow characteristics of
electromagnetically-stirred melt in the mushy zone is critical in order to control the grain
structure of cast alloys.
Electromagnetic (EM) stirring is generally accomplished by induction from a time-
varying magnetic field using a suitable induction coil. The passage of an alternating current
induces eddy currents in the melt, which are dissipated as heat (Joule heating). Also, the
interaction between the induced current and the applied magnetic field produces EM forces,
which drive the flow in the melt. The flow behavior in EM stirred melts is generally controlled
by the applied magnetic field

Recommended